The Journal of Physical Chemistry, Vol. 82, No. 6, 1978
R. G. Herman and D. R. Flentge
halide crystal^.'^^^^ The comparison shows that, from the point of view of their central-atom hyperfine interactions, which are isotropic and of magnitudes comparable to those of T l F t - and PbFl-, a molecular description is entirely appropriate. The anisotropy in the “ligand” hyperfine interaction also favors a molecular description. For this reason we have included in Table I1 data for Si3+in LiFa2I Its 19Fhyperfine anisotropy is quite compatible with the other data when converted to a F(2p) contribution to the SOMO, although it is regrettable that no 29Sihyperfine satellites could be detected for pecies. A prediction of the 29Sihyperfine interactio be made from Table I1 and the MWHS atomic par l4 -3700 f 300 MHz. The failure21to detect 29Sisignals in samples where the signal/noise ratio for the main spectrum was -1OO:l casts doubt on the identification of silicon as the impurity element.
J. R. Morton, K. F. Preston, and J. C. Tait, J . Chem. Phys., 62, 2029 (1975). A. R. Boate, J. R. Morton, and K. F. Preston, Chem. Phys. Lett., 50, 65 (1977). A. R. Boate, J. R. Morton, and K. F. Preston, J . Chem. Phys., 67, 4302 (1977). R. P. Graham, J. Macnarnara, I.H. Crocker, and R. B. MacFarlane, Can. J . Chem., 29, 89 (1951). D. H. Brown, K. R. Dixon, R. D. W. Kemmitt, and D. W. A. Sharp, J. Chem. Soc., 1559 (1965). G. Wagner and H. Binder, 2.Anorg. Allg. Chem., 297,328 (1958). R. Hoppe and K. Blinne, 2.Anorg. Allg. Chem., 293, 251 (1958). A. R. Boate, J. R. Morton, and K. F. Preston, J. Magn. Reson., 23, 259 (1976). G. Breit and I. I. Rabl, Phys. Rev., 38, 2082 (1931). J. E. Nafe and E. B. Nelson, Phys. Rev., 73, 718 (1948). J. R. Morton and K. F. Preston, J . Magn. Reson., In press. F. Herman and S. Skillman, “Atomlc Structure Calculations”, Prentlce-Hall, Englewood Cliffs, N.J., 1963. J. H. Mackey and D. E. Wood, J. Chem. Phys., 52, 4914 (1970). P. W. Atklns and M. C. R. Symons, ”The Structure of Inorganic Radicals”, Elsevier, Amsterdam, 1967, p 103. A. R. Boate, J. R. Morton, and K. F. Preston, Proceedlngs of the V I International Symposium on Magnetic Resonance, Banff, Canada (J. Magn. Reson., in press). W. Dreybrodt and D. Silber, Phys. Status Solidi, 20, 337 (1967). D. Schoemaker and J. S. Kolopus, Solid State Commun., 8, 435 (1970). J. Dugas, DSc. Thesis, University of Toulouse, 1970.
References and Notes NRCC No. 16514. NRCC Research Associate 1975-1977, A. R. Boate, J. R. Morton, and K. F. Preston, J. Phys. Chem., 80, 2954 (1976).
Electron Paramagnetic Resonance Parameters of Copper(I1) Y Zeolites Richard G. Herman”” and Dennls R. Flentgelb Department of Chemlstry, Texas A&M University, College Station, Texas 77843 (Received July 25, 1977)
The number of electron paramagnetic resonance (EPR) parameters for copper(I1)ions held in lattice positions in dehydrated low exchanged sodium Y zeolites, as well as the relative intensity of each set of g values observed in the spectrum, was found to vary as a function of evacuation time at ambient temperature prior to activation. The usual procedure of evacuating the sample for 15-60 min before beginning the thermal treatment in hourly increments resulted in the following parameters for low Cu(I1) exchanged Y zeolites: gill = 2.38(110),g,l = 2.06(20), g1I2= 2.30(175), gL2= 2.03, and in some cases g1l3 = 2.36(125), where the numbers in parentheses are the observed hyperfine splittings (in Gauss). Prolonged evacuation of the low Cu(I1) ion exchanged Y zeolites yielded gill = 2.37(125),g,l = 2.06(20),g1I2= 2.32(160),and gL2= 2.03 following dehydration to 400-500 “C. Parameters similar to the latter values were obtained for highly ion exchanged Cu-Y zeolites following partial reduction with hydrogen or carbon monoxide, as well as upon partial reoxidation of the latter samples with oxygen or nitric oxide. The second set of EPR parameters is attributed to copper(I1) ions located in sites in the small cages, while the gl and g2subsets of the first group are due to copper(I1) ions localized in the zeolite supercages. Most of these sites provide a distorted trigonal environment for the divalent copper ions. By correlatingthe zeolite treatments reported in the literature to the present results, the disparity among previously given EPR parameters for Cu(I1)-Y zeolites can be explained in most cases.
Introduction Metal cation exchanged zeolites are successful catalysts for a wide range of chemical reactions. The metal atoms or ions are the active sites, and many of those having unpaired electrons have been characterized by electron paramagnetic resonance (EPR). The resultant spectra have been used to interpret the oxidation states of the lattice-held ions and the degree of complexation by various ligands. Of current interest are the transition metal ion exchanged zeolites, and the systems consisting of the first row transition metal ions in Y lite, viz., chromium,2 manganese,3p4i r ~ n ,~~otb~a l t , ~ - ~e1,2J0and copper,10‘22 have been the most intensively studied by EPR. Because of the numerous lattice sites that these ions can occupy, speculation as to the location of these cations in the 78/2082-0720$01.0010
dehydrated Y zeolites, with the exception of Mn(II),334is not usually made. It is generally accepted that the cations in the hydrated zeolites exist as rather free aquo complexes located mainly in the supercages of the zeolite structure. Unfortunately, little EPR data have been obtained for transition metal containing A zeolites. Due to the simplicity of the A zeolite structure, there are only three nonequivalent sites occupied by monovalent cations, but only one of these general sites (in or near the six rings) usually stabilizes divalent cations.23 By using diffuse reflectance spectroscopic methods or single crystal x-ray structure determination techniques, the location of Cr(II),= MII(II),~~ C O ( I I ) , and ~ ~ , Ni(II)28 ~~ in dehydrated A zeolites has been asserted. The bare cations are found to be located near the center of the six-ring windows and to be 0 1978 American Chemical Society
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978 721
EPR Parameters of Cu(I1)-Y Zeolites
TABLE I: Experimental EPR Parameters Reported for Copper(I1) in Dehydrated Low Ion Exchanged Y Zeolitesaib % Cu(I1) exchanged 1 2 4 4 5 7 10 11 14
2.35(120) 2.38(108j 2.386( 130) 2.37(120) 2.38( 107) 2.26(130) 2.38(130)
2.084(16) 2.07(22) 2.06' ' 2.062(20) 2.06(13)
2.325( 160) 2.33(170)d 2.31(175) 2.30('175 j 2.323(176) 2.32(1601 2.30( 175j 2.32( 154) 2.31(153) 2.346(160)d 2.328( 171)d 2.32(162) 2.30(175)
2.06 2.058 2.048(24) 2.06
Ref 11 12 13 14 15 16 17 18 19 20 21 22 14
2.071 ( 16.4)d>e 14 2.06( 26)d 2.382(137)d 2.077 ( 15)d 14 2.05(22) 2.08 14 2.38(126) c C 2.38(108) 17 a The dehydration procedures used are as follows in order of reference numbers: (11)heat at 383 K in air for 8 h, increase temperature to 473 K for 8 h, and then heat in 0, at 673 K for 72 h; (12) heat at 673 K ; (13) heat at 423 K; (14) evacuate and then heat to 6 7 3 K stepwise under a dynamic vacuum; (15) evacuate a t 343 K; (16) evacuate overnight and then heat to 773 K; (17) evacuate 1 h and then heat to 773 K stepwise under a dynamic vacuum; (18) evacuate at 373 K, add O,, and then evacuate stepwise to 773 K ; (19) not given; (20) evacuate and then activate stepwise to 673 K under a dynamic vacuum; (21) heat to 623 K and evacuate 2 h ; and (22) evacuate and heat to 472 K in 4-5-h under a dynamic Numbers in parentheses are the observed hyperfine splittings (in Gauss unless stated otherwise, 1 G = 1.070 X vacuum. Hyperfine splitting is given in units of lo4 cm-'. e A l o 4 (g,!g) cm-'). Observed, but the g value was not given. strong line at g 2.05 was also observed.
TABLE 11: Chemical Composition (mequiv g-') of the Hydrated CuY Zeolites Cu(I1) Sample
Na + Calcd"
Cu(I1) ions per unit cell
CUY-0 0.000 0.000 3.21 3.21 0.0 0.0 CUY-1 0.033 0.032 3.16 3.18 1.0 0.3 CUY-2 0.068 0.070 3.07 3.13 2.2 0.6 CUY-4 0.136 4.3 1.2 CUY-10 0.316 0.314 2.90 2.89 9.8 2.7 CUY-17 0.555 17.4 4.9 CUY-32 1.028 32.0 9.0 CUY-60 1.932 60.2 16.9 CUY-68 2.167 2.170 1.03 1.03 67.8 19.0 a The values were calculated from the chemical composition of the parent NaY zeolite and the percent copper(I1) (column 6). The degree of hydration was found to be approximately the same €or all of the samples (= 260 H,O/unit cell).
coordinated to three oxygens in the ring. This results in the approximate D3h ligand field symmetry around the cations. This symmetry, as well as others, is also possible to attain in the Y zeolites. X-ray structure determinations have been carried out for a dehydrated Cu(I1)-Y zeolite (from powder photograph^)^^ and for hydrated and dehydrated Cu(II)-fa~jasite.~~ In both studies, it was found that the copper(I1) ions strongly preferred site I' (site I'A in the latter work), which has approximately D3h symmetry. No attempt has been made to correlate the structural data with EPR results. This might be due to the great variance (shown in Table I) between EPR parameters obtained by different research groups working with similar Cu(1I)-Y zeolites. It should be noted that the structural studies made use of highly exchanged zeolites, while most EPR investigations used low exchange levels so that the paramagnetic ions were distributed widely enough to prevent the pairing of copper spins. The present study was undertaken to correlate sample treatment with the resultant EPR parameters, to clarify the assignment of the parameters to the spectra, and to extend our knowledge of actual copper(I1) ion locations in low exchanged Y zeolites. Experimental Section Materials. CuNa-Y samples with various Cu(I1) contents were prepared from a Llnde Na-Y zeolite (lot no. 13544-76). This zeolite was ion exchanged with Cu(N03)2.3H20solutions of different concentrations in order
to obtain samples with different Cu(I1) contents. The general procedure was to add the zeolite to the Cu(I1) solution such that the ratio of solution to solid was 20 cm3/g, stir continuously for 4 h at ambient temperature, and then filter the solution and wash the collected zeolite 10 times using a total of 20 cm3 of H20/g of solid. The zeolite was subsequently dried a t ambient temperature in an open vessel placed in a fume hood. The C U ( N O ~ ) ~ content of the solution determined the final solution pH, as well as the amount of Cu(I1) ion exchanged into the zeolite, e.g., 0.01 M Cu(I1): pH 7.1 and CuY-10. The samples are denoted as CuY followed by a figure showing the exchange level of Cu(I1) in percent of the total cation exchange capacity. The CuY-2 sample was prepared from a zeolite-0.01 M Cu(I1) solution that was made alkaline by the addition of 0.1 M NaOH (final pH 9.0). CuY-68 was obtained by equilibrating the zeolite consecutively with two portions of 0.10 M Cu(I1). The composition of the samples is given in Table 11. The copper(I1) concentrations were determined by atomic absorption measurements following back-exchange of the zeolites by Ag(1). The sources and purification of the gases used have been previously reported.17 Sample Treatments. In the usual activation procedure, the zeolites were degassed to either 400 or 500 "C under vacuum Torr) in a conventional EPR batch cell (cell volume to zeolite mass ratio -200 cm3/g). The temperature was raised hourly in 100 "C increments after first evacuating the cell for 0.5-1 h at room temperature. Following this, oxidation was usually carried out at the
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978
maximum dehydration temperature with 50-400 Torr of O2 for a short period of time. This treatment was usually applied to samples prepared as thin platelets,14 but identical EPR parameters were obtained when the treated zeolites were in powder form. Three of the Cu-Y zeolites were subjected to prolonged Torr) at ambient temperature dynamic evacuation ( before being thermally dehydrated using the temperature programming given above. Following various periods of the initial evacuation, the samples were cooled to 77 K and EPR spectra were obtained. After warming to room temperature, the evacuation was continued. Water vapor was added to the samples in 20-Torr portions following the thermal activation. In this series of experiments,powdered zeolites were used. In another set of experiments, the samples were subjected to various reduction and reoxidation treatments after dehydration. In the Results section, reference will be made to the following reduction procedures: (I) activate to 500 "C and reduce with 50 Torr of H2 at 500 "C for 3 h; (11)reduce with 300 Torr of H, at 500 "C for 18 h; (111) dehydrate to 400 "C, oxidize with 50 Torr of O2 for 0.25 h at 400 "C, and reduce three times with 300 Torr of H2 for 1 h at 200 OC; (IV) dehydrate to 200 "C and reduce at 200 "C with 300 Torr of H, for 2 h; (V) activate to 400 "C and reduce with 400 Torr of H2 at 200 "C for 0.25 h; (VI) dehydration to 500 "C, equilibration with 300 Torr of CO at 500 "C for 3 h, evacuate 2 h and equilibrate with 23 Torr of NO for 2 h, evacuate and add 265 Torr of CO at 500 "C, equilibrate for 2 h and then evacuate 0.5 h; (VII) dehydration at 400 "C and reduction by six treatments at 400 "C with 400 Torr of CO (total reduction time 66 h); and (VIII) oxidize with 500 Torr of 02,evacuate, and then reduce with 300 Torr of CO at 500 " C for 3 h. The reoxidation treatments used were the following: (IX) heat for 3 h at 500 "C in the presence of 50 Torr of 0,; (X) oxidize with 300 Torr of O2 at 500 "C for 18 h; (XI) equilibration with 20-22 Torr of NO at ambient temperature; (XII) add 43 Torr of NO and equilibrate at ambient temperature for 14 h; and (XIII) equilibration with 30 Torr of NO at 25 "C for 0.5 h. EPR Spectroscopy. The EPR spectra were obtained at 77 K with a Varian E-6S spectrometer equipped with a TElo2mode cavity as described previ0us1y.l~The g values are reported relative to a 2,2-diphenyl-l-picrylhydrazil (DPPH) or phosphorus-doped silicon standard or to a sample of pitch in KCl. Usually the estimated error in the g values is k0.005 and in the hyperfine splittings is f 2 G. However, the estimated errors in the parameters for CuY-1 and CuY-2 are approximately double these figures. Spin concentrations were determined by numerical double integration of the spectra and comparison to a reference spectrum obtained with a single crystal of copper(I1) sulfate.
Results The preparation of Cu-Y zeolites by ion exchange in aqueous media is a rather straightforward procedure, but a diverse range of treatments can be used to prepare the materials for subsequent chemical, spectroscopic, and catalytic studies. In the present work, the influence on the resultant EPR parameters of CuO in or on a Cu-Y zeolite will be described. The changes in the EPR parameters, especially the parallel hyperfine splittings, obtained for activated Cu(I1) ion exchanged Y zeolites for which the duration of evacuation at ambient temperature prior to dehydration was varied will be presented. These parameters will be compared with those obtained by partial reduction of the copper ions with hydrogen or
CuY.10 g L
3 I 3120
_ -- - 0 -
OF EVACUATION (hr)
-2 0 065
I n 500
Figure 1. The varlation of magnetic field position of the g L hyperfine lines of CuY-10 as a function of sample treatment. The final treatment consisted of equilibration with water vapor for 1 h followed by evacuation at 295 K for 46 h. y is the maximum estimated error (see the Experimental Section) in the g values, several of which are designated by arrows.
carbon monoxide and with those observed after partial reoxidation of the zeolites by oxygen or nitric oxide. Cu-2 Containing CuO. The air-dried Cu-Y zeolites, except CuY-2, were all light blue with a gradation from nearly white (CuY-1)to a definite blue (CuY-68). CuY-2 was a light brown or tan in color. This sample had been prepared in a solution where the pH had been artificially adjusted to a value of 9, and this resulted in the precipitation of the copper that remained in solution following partial exchange of the zeolite. The initial color of the precipitate was light blue, but the color turned to light brown upon air drying at slightly higher than ambient temperature. The zeolite did not change color upon back-exchange overnight in the dark at approximately 70 "C with silver ions. The tan color is assumed to be due to CuO, probably in a hydrated state, formed in or on the zeolite. The quantity of this oxide was calculated to be about 0.012 g/g of anhydrous zeolite, but an x-ray powder diffraction pattern of the hydrated sample failed to demonstrate the presence of any crystalline CuO. A portion of anhydrous Na-Y mixed with black 100% CuO (Baker Analyzed) in the proportions given above gave a diffraction pattern of CuO that could be seen only very faintly above the background. The appearance of the mixed sample was an off-white light grayish color. Upon activation of the ion exchanged zeolite sample, a dark grayish color resulted and a set of weak lines corresponding to CuO was detected in the x-ray diffraction pattern of the sample. The presence of CuO in or on the CuY-2 zeolite did not interfere with the EPR analysis of the lattice-held divalent copper ions. Evacuation and Thermal Treatments. A wide variety of activation (dehydration) procedures had been previously employed for Cu-Y zeolites, as is evident from Table I. Some of those involved long periods of evacuation prior to heat treatment, while others used short evacuation or even no evacuation at all. Therefore, the effect of varying the duration of evacuation previous to the activation was studied. The air-dried low exchanged Cu-Y zeolites exhibited one set of g values with no hyperfine splitting (designated as !AI) observed in the g, region. Upon evacuation at ambient temperature, a second set of EPR parameters arose, and following prolonged evacuation this became the dominant set. As indicated in Table 111,g L 2 consisted of a single strong line. This line became more intense than the g,l signal by 6 h of evacuation for CuY-1 and by 18 h of evacuation for CuY-10. Figure 1indicates
The Journal of Physical Chemistty, Vol. 82, No. 6, 1978 723
EPR Parameters of Cu(I1)-Y Zeolites
TABLE 111: Experimental EPR Parametersa Obtained for Cu(11)-Y Zeolites upon Prolonged Evacuation Treatment 1 min 2h 27 h 92 h 100 'Cy 1 h Activated t HzOe 18 h 1min 0.75 h 15 h 40 h 65 h 184 h Activate f t H,Oe 16 h 40 h
1 min 1.5 h 18 h 103 h 219 h 306 h 465 h 100 'C, 1 h Activate f i g
A. CUY-1 2.042' 2.057(14) 2.057( 1 6 ) 2.057(18) 2.059(17) 2.059(16) 2.060(18) 2.055 (18)
2.332(150) 2.324(150) 2.320(150) 2.336( 150)
2.029 2.025 2.025 2.023 2.021 2.022 2.024
2.318( 160) 2.314(162) 2.306(165) 2.305( 166) 2.311(155)
2.033 2.030 2.030 2.028 2.025 2.025
2.36(135) 2.364( 120) 2.363( 123)
B. CUY-2 2.051' 2.063( 18) 2.065( 18) 2.067(19) 2.064(19) 2.060( 19) 2.065(1 6 ) 2.05' 2.062(17) 2.061(17)
2.314( 160) 2.307(168)
2.393(121) 2.370(124) 2.365(121) 2.367(120) 2.369(121) 2.377( 120) 2.376( 118) 2.377(122) 2.378(124) 2.392(130) 2.372(119)
c. CUY-10 2,053' 2.055' 2.063(18) 2.064(20) 2.069(21) 2.074(23) 2.074(23) 2.061(20) 2.060( 20) 2.056' 2.056( 20)
2.313(162) 2.316(160) 2.320(159) 2.328(158) 2.325(158) 2.326(161) 2.325(164)
2.026 2.026 2.031 2.034 2.034 2.028 2.025
2.371(120) 2.373(122) 2.364(120) 2.342(138) 2.377(122)
2.360(136) 2.369(122) 2.372( 120) 2.372(120) 2.369(120) 2.361(123)
2.011 2.017 2.013 2.013
2.320(161) 2.027 Time listed is the total duration of evacuation a Numbers in parentheses are the hyperfine splittings (given in Gauss). Heated to 673 K stepwise at ambient temperature. 'The given g value indicates the center of the perpendicular signal. under a dynamic vacuum, oxidized at 673 K for 5 min with 400 Torr of 0 , , and then evacuated for 1h at the same temperature. e Equilibrium water vapor pressure = 20-22 Torr; equilibrate for 1 h. f Heated to 773 K stepwise under a dynamic vacuum. g Oxidized for 2 h at 773 K with 50 Torr of 0, and then evacuated for 68 h.
Flgure 2. The EPR spectra obtalned at 77 K for CuY-10 after being evacuated at ambient temperature for 465 h (A) and then subsequently being activated at 773 K (B) using the stepwise dehydratlon procedure. The sharp line at high field is due to the phosphorus-doped silicon that was used as a g value marker.
that for CuY-10 the gL2signal appeared (as a shoulder) before the g,l line was split by hyperfine interactions, which occurred after 18 h of evacuation. From Table 111, it is evident that the value of gL2decreased slightly for CuY-1 and CuY-2 as evacuation proceeded. However, it increased for CuY-10, and this increase was accompanied by the appearance of an additional line in the g, region. This latter signal (gL2) appeared after about 48 h of evacuation and grew from a shoulder to the most intense line within 15 h. After 200 h of evacuation, gL2was a weak signal that almost disappeared as is shown in Figure 2A. In general, only a slight shifting of the EPR parameters occurred during the evacuation at 25 "C, but definite changes were noticed in the spectra upon activating the samples to 400-500 "C. The spectrum obtained upon activation of CuY-10 is given in Figure 2B, and the EPR parameters are listed in Table IIIC. Upon rehydration, the sets of g values collapsed into one set and the spectra resembled those of the starting hydrated zeolites. For CuY-1 and CuY-2, the Mn(I1) that was present in the samples as an ion exchanged impurity produced a spectrum (in particular, the first line of the six-line spectrum) which was observable after the rehydration, while for the initial samples it was observable only with CuY-1. The EPR parameters of the three activated samples (see Table 111) were quite different. In contrast, Table IV shows that activation of low exchanged Cu-Y zeolites at 400-500 "C after a brief evacuation yielded g and IAI values
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978
R. G. Herman and D. R. Flentge
TABLE IV: g Values and Hyperfine Splittingsa (in G ) for Cu-Y Zeolites Dehydrated at 400-500 "C Following a Brief Period of Evacuation (< 1 h ) Sample 811I gii* 811 CUY-1 2.378(108) CUY-2 2.380(110) CUY-4 2.380(110) 2.300( 175) CUY-10 2.383(108) 2.308(174) 2.36(123) CUY-17 2.386(108) 2.300(175) 2.36(125) a The numbers in parentheses are hyperfine splitting values. The g value
that were nearly identical. In addition, the parallel hyperfine splittings belonging to the most intense lines (gill and g 2, were entirely different from the splittings listed in Ta le 111. Magnifying the spectra by increasing the receiver gain of the spectrometer resulted in the detection of a third set of hyperfine splittings (All3). The evacuation technique used was particularly important in determining the EPR parameters. For example, following the evacuation of CuY-10 for only 2 min and then allowing the sample to stand at ambient temperature for 23 h, EPR analysis yielded gll = 2.379(131) and g, = 2.056, where the number in parentheses is the hyperfine splitting in units of Gauss. After activation to 500 "C, the spectral parallel components were glll = 2.371(121) and gli2 = 2.304(158), which are approximately the same parameters as those obtained following prolonged evacuation and subsequent activation. Reductions with Hydrogen. The above zeolite sample was reduced using reduction procedure I, and the resulting spectrum is shown in Figure 3A. The Cu(I1) concentration was calculated from the spectrum to be approximately 0.15 Cu(II)/unit cell (corresponding to CuY-0.5), and the EPR parameters were observed to be glll = 2.364(121), g,l = 2.060(20),g ? = 2.324(160),and gL2= 2.025. The low-field (mI= -3/2\ components of the two g values appeared to be resolved, and this agreed with the hyperfine splittings indicated. However, the resolution might be due to or enhanced by resolved hyperfine splittings for the 65Cu isotope (31% abundance) that are approximately 7% larger than the splittings due to 63Cu, although such resolution is not noted for the high-field parallel components. From the g, lines, it is apparent that the gl signal was more intense than the g2 line. Upon evacuation for 26 h at ambinet temperature, the entire spectrum decreased in intensity. In addition, the g L 2line decreased greatly in intensity while a signal (gL3)at g = 2.017 grew to be about as strong as gL1. No particular change in the gll region of the spectrum was evident. Reoxidation using procedure IX led to complete restoration of the activated Cu(I1)-Y spectrum with EPR spectral components in the parallel region of Ail1 = 120 G and All2 = 160 G. A fresh portion of CuY-10 was evacuated briefly and then activated at 500 "C, and the resultant spectrum yielded the EPR parameters given in Table IV. The sample was then reduced using reduction procedure I1 and reoxidized after evacuating for 0.25 h at the elevated temperature by using reoxidation procedure X. The reduced sample was bright reddish-pink (x-ray powder diffraction demonstrated the presence of metallic copper crystallites having diameters of at least 30 nm when another portion of CuY-10 was activated and reduced using the same procedure) and did not exhibit an EPR signal. The reoxidation converted 74% of the copper to divalent copper held in lattice sites, as determined from the intensity of the EPR spectrum, and the EPR parallel parameters of the reoxidized zeolite were gill = 2.380(109) and gl12 = 2.302(172). After subjecting the sample to reoxidation procedure X for a second time, an EPR spectrum
2.044(21) 2.039(18) 2.049(21) 2.060( 20) 2.058( 20)
2.055(17) 2.051(15) 2.060(18) 2.073( 19) 2.059(20)
2.027 2.022 2.030 2.040 2.037
is obtained from the center of the line.
c i 200 0
Figure 3. The EPR spectra of hydrogen reduced samples of (A) CuY-10 and (6) CuY-68 that were treated as follows: (A) reduction procedure I after equlllbratlng in vacuo for 23 h and (B) reduction procedure 111.
with unchanged parameters was obtained with an intensity equivalent to 92% of that obtained with the initial activated sample. Although the sample appeared light gray, x-ray diffraction analysis failed to show the presence of CUO. After evacuating for 1h at room temperature, a sample of CuY-68 was reduced using reduction procedure 111,and the H2 was then evacuated at 200 "C for 0.25 h. The EPR spectrum shown in Figure 3B was obtained, where the calculated Cu(I1) concentration was 0.4 Cu(II)/unit cell (equivalent to CuY-1.4), and the experimental parameters were gill = 2.361(126), gL1 = 2.059(20), g1I2 = 2.315(155), and gL2= 2.023. The latter set of g values was the more intense set and no evidence of gL3 = 2.017 was found. After recording the above spectrum, the sample was completely reduced a t 400 "C with hydrogen and then reoxidized for 5 days according to procedure XI. The subsequent EPR spectrum indicated the Cu(I1) content at lattice sites to be equivalent to CuY-1.5; the observed parameters were g = 2.371(125), gL1 = 2.066(19), g1I2 = 2.322(156), and gLi = 2.033. The same parameters were obtained by reduction of CuY-68 according to procedure IV following a 1-h evacuation. A sample of CuY-60 was activated to 500 OC, completely reduced using reduction procedure 11, and evacuated for 1 h at the elevated temperature. After adding oxygen at approximately 450 "C, reoxidation procedure IX was carried out. A t the given pressure of oxidant, less than 50% of the copper was reoxidized to Cu(I1). The resultant EPR spectrum indicated that approximately 50% of the
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978 725
EPR Parameters of Cu(I1)-Y Zeolites
TABLE V: EPR Parameters4 for the Spectra of CuY-10 Shown in Figure 4 2.083b A 2.374(126) B 2.385(109) 2.054(13) 2.051(13) 2.305(172) 2.025b C 2.385(109) 2.052(13) 2.304(170) 2.025b 2.367(122) D 2.380(110) The g value indicates the center of the The numbers in parentheses are the hyperfine splittings (in Gauss). perpendicular line. g(hyd)
Figure 4. The EPR spectra of CuY-10 observed after the following consecutive treatments: (A) evacuation at 298 K for 0.5 h; (B) reduction procedure V I and reoxidation procedure XII; (C) heating at 473 K for 0.5 h; (D) evacuation for 0.5 h at 473 K and then 0.5 h at 573 K; (E) evacuation at 773 K for 16.5 h; and (F) reoxidation procedure XIII.
reoxidized copper existed as spin-paired copper ions with gi = 2.16 and with the remaining copper ions having spectral parallel components of 128 G (All') and 159 G (All2). For comparison, CuY-32 was reduced to CuY-17 using reduction procedure V. The EPR parameters were gill = 2.359(124),g,' = 2.059(20),g1I2= 2.306(157), and gL2 = 2.022, where the g' set was more intense than the g2set. The g,, values corresponding to the g' and g2 sets of parameters for the three partially hydrogen-reduced samples were 2.160 f 0.001 and 2.121 f 0.004, respectively, where g,, = + 2gJ/3. Reductions with Carbon Monoxide. The partial reductions described above were carried out using hydrogen gas as the reducing agent, while the following reductions were carried out using carbon monoxide so that water could not be formed. After evacuating for 0.5 h, CuY-10 was reduced using procedure VI and reoxidized by procedure XII. The spectra obtained for the gil region are shown in Figure 4. No Cu(I1) signal was observed after the reduction and, although the sample was white, the distinctive EPR spectrum of the Cu+-NO complex3' was not apparent upon the addition of NO as the oxidant. The reasons for this have been discussed e1~ewhere.l~The signal marked by the light vertical line in Figure 4 is the first line of the Mn(I1) spectrum. The amplifications of spectra B and C and of spectra D, E, and F are approximately 64 and 51 times, respectively, that of spectrum A. The set of splittings corresponding to g113disappeared upon addition of NO but reappeared upon equilibration for 3
Figure 5. The EPR spectra of CuY-60 following stepwise activation to 773 K (A), oxidation with 02, and subsequent reduction with CO at 773 K for 3 h (B).
days, Following a 0.5-h heat treatment a t 200 "C, mass spectrometric analysis showed that part of the NO had been converted into N2 (along with a small quantity of N20). After evacuation of these gases, g1l3 was quite pronounced. The EPR parameters of the spectra in Figure 4 are listed in Table V, and it can be noted that two g, values were observed, but a third could not be discerned. Reducing a CuY-60 sample using reduction procedure VII, a sample corresponding to CuY-2.4 was obtained that exhibited the following EPR parameters: g = 2.378(123), 8,' = 2.073(20), glt = 2.325(159), and gLJl= 2.035. The intensities of the two sets of g values were approximately equal, and the spectrum indicated that no spin-paired copper was present. This sample was then completely reduced with CO at 500 "C and subsequently reoxidized using procedure XI. After 20 h, a Cu(I1) EPR signal was barely visible above the very strong Cu+-NO spectrum. After standing for 68 h, an evacuation was carried out for 2 h, which destroyed the Cu+-NO complex and yielded a Cu(I1) signal proportional to that of CuY-3. The two sets of parameters of similar intensity were gill = 2.378(123), g', = 2.071(19), g112 = 2.320(155), and gL2= 2.038. Beginning with a fresh sample of CuY-60, activation was carried out to 500 "C after a 1-h evacuation period. The resultant EPR spectrum was typical of Y zeolites highly exchanged with Cu(I1) (gi = 2.16) and is shown in Figure 5A. Reduction procedure VI11 was then carried out, and spectrum exhibited in Figure 5B was subsequently obtained. The indicated hyperfine splitting values were All1 = 128 G and All2*=154 G, while the isotropic line demonstrated that spin-paired copper ions were still present. Analysis of the gas phase over the reduced zeolite by mass spectrometry showed that COz had been formed during
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978
the reduction. The remaining Cu(I1) ions were reduced by two more CO treatments and then reoxidation procedure IX was applied. The intensity of the EPR spectrum that resulted was intermediate between those of the spectra in Figure 5, while the A values observed after the first CO reduction were regenerated. Spectrum 5B approximates those obtained by partial reduction and partial reoxidation of CuY-60 using hydrogen.
Discussion Evacuation of Cu-Y Zeolites. Upon evacuation of the low exchanged zeolites, e.g., CuY-1, CuY-4, and CuY-10, for 1min to remove oxygen from the sample cell, a rather uniform set of EPR parameters were usually obtained, viz., gil = 2.38 f 0.01, g, = 2.05 f 0,001, and All = 122 f 3 G. However, as observed in Table 111, a hyperfine splitting of 136 G was found for CuY-2, but upon further evacuation the value decreased to approximately 120 G. Upon repeating the experiment with a fresh portion of CuY-2, identical results were obtained. Similar high initial splittings for CuY-10 and CuY-32 were obtained (135 G in each case) by evacuating the sample cell for only 0.25 min instead of 1min. The latter hyperfine splitting value was also observed for these materials when the evacuation step was eliminated. Therefore, the presence of CuO in or on CuY-2 seemed to influence the hyperfine splitting value observed in the EPR spectrum after a brief evacuation, perhaps by hindering and delaying the removal of water from the supercages of the zeolite. The set of parameters with values of gl, = 2.38(135),g, = 2.05, and g, = 2.16 is assigned to the hexaaquocopper(I1) complex. For comparison, Cu(H20),2+in a 60% glycerine-40% water mixture a t 253 K was found to have g,, = 2.199 with gll = 2.400( 137) and g, = 2.099( 13).32It is evident that the present experimental g,, value is lower than the frozen solution value,32and it is also lower than the g,, values of 2.192 and of 2.194 attributed to the hexaaquo complex exchanged into Dowex 50W.33334 Evacuation of the zeolites for 1-2 h resulted in the anisotropic spectrum with the approximate EPR parameters of gli = 2.37(122), g, = 2.06(18), and g, = 2.16. This spectrum might be due to Cu(I1) ions in a more-or-less square based penta-coordinated environment. Upon prolonged evacuation, a third set of parameters arose (see Table 111)with g,, = 2.12-2.13. This set is attributed to the tetraaquocopper(I1) complex, and the g, value can be compared with that of g,, = 2.135 for the square-planar Cu(NH3)?+ complex in Y ze01ites.l~The aquo complexes were not observed to be in a solution-like environment in these zeolites insofar as dynamic Jahn-Teller distortion^^^ and rapid tumbling36did not average the anisotropy nor appreciably broaden the spectra even at room temperature. It should be pointed out that g,, is the pseudoisotropic value of gi that would be found a t ambient temperature in solution when the viscosity is such as to allow the molecules to tumble freely. This assumes that no change in structure or bond lengths occurs upon freezing. Addition of axial ligands to a square-planar copper(I1) complex leads to an increase in the value of g and a decrease in All (when the magnitude of All is negative, as it is for most copper(I1) complexes). Considering the parameters observed for the hexaaquo and tetraaquo complexes, values of gli = 2.35-2.38 and All I 160 G would be expected for a square-pyramidal-type of pentaaquocopper(I1) complex. Considerable error might be involved in these estimates because the fifth ligand would tend to pull the copper ion out of the plane of the four equatorial ligands, and this should result in a decrease in the in-plane bonding strength, which would lead to an increase in the N
R. G.Herman and D. R. Flentge
g values. The effect on the hyperfine splittings is less certain. Analogous to this treatment would be the situation where one of the weak axially coordinated water ligands would be replaced by a stronger ligand. This might be the case if the pentaaquo complex were attracted to the zeolite skeletal wall in the sixth coordination site, such as might occur when much of the zeolitic water is removed by evacuation at ambient temperature for a short time. Thus, in fact, the Cu(I1) ion is probably still six coordinate, but the interaction with the zeolite results in nonequivalent axial ligand fields and produces a pseudo-five-coordinate environment around the copper ions. In addition to the EPR parameters attributed to the aquo complexes, a symmetric line a t g = 2.27 with a peak-to-peak width of =lo0 G appeared after evacuating CuY-2 for about 15 h. This line grew in intensity for the next 50 h, after which the intensity became constant. This g value is the same as that reported for C U O . ~Upon ~ activating the zeolite to 500 "C for 3 h under a dynamic vacuum, the signal disappeared but reappeared after rehydration of the sample with water vapor. These observations indicate that the symmetric line should probably be attributed to a disordered surface species such as [Cu(OH),12-" or [Cu(H20),l2+rather than to CuO. A symmetric line such as this was not evident with CuY-1 nor with CuY-10. Activated and Reduced Cu-Y Zeolites. Figures 1 and 2A indicate that upon prolonged evacuation of CuY-10, three g, values were observed. Subsequent activation resulted in spectrum B of Figure 2, where the g, portion of this spectrum is identical with the spectrum obtained by dehydration following a brief evacuation period (values given in Table IV), and an illustration of the latter spectrum is given e1~ewhere.l~The g, value is usually quoted to be e2.06 (see Table I), but in reference to Figure 1 and the spectra in Figure 2 it seems evident that two g, values should be assigned instead, and these would correspond to the g, values of the two strongest signals observed for the thermally activated samples. This would result in the g, value given in Table IV to be converted from g, = 2.05 f 0.01 to g,l = 2.06 f 0.01 and gL2= 2.03 f 0.01. The two weak high field lines in Figure 2, as well as a line near the third gill line (mr = +1/2) result from a monoaquo- or diaquocopper(I1) complex that will not be discussed here. A strong gL3line is evident in Figure 2A, although a set of corresponding g1l3lines differing from glll and g1I2 was not observed. Considering the data in Table 111,g113 and All3must approximate the g1I2parameters, e.g., g113 = 2.32 and All3 = 155 G. Upon activation, the gl parameters changed very little but gL3disappeared and g,2 a growth in intensity. In addition, there is a diminution in the overall EPR intensity. Since gill, g1i2,All1, and All2 change very little in magnitude, especially for CuY-10, similar symmetries surrounding the Cu(I1) ions are indicated for the evacuated and the activated zeolites. Upon rehydration, the copper(I1)-hexaaquo complex was easily re-formed, and the loss in EPR intensity was regained. Activation following a brief evacuation resulted in different EPR parameters, which were given in Table IV. Under these conditions, the zeolites proceed from a hydrated state to a dehydrated state rather quickly, and it might be expected that most of the Cu(I1) ions would be rapidly stripped of their waters. The parameters of gill = 2.38(110) and g,l = 2.06(18) for the resultant zeolites demonstrate that the Cu(I1) geometry is axial and is either (a) of a type between square-coplanar and tetrahedral, (b) a square-pyramidal configuration, or (e) a rhombically or
EPR Parameters of Cu(I1)-Y Zeolites
tetragonally elongated octahedral configuration with the A Cu(I1) complex having rather strong covalent ion in a square-coplanar environment would be expected to have a much greater IAill value. In case (a), IAI would indicate the symmetry to be analogous to compressed tetrahedral, such as that observed for copper-doped dichloro(l,10-phenanthroline)zinc39 and dichloro(sparteine)~inc(II),~O for which gil = g, = 2.297(123) and 2.299(90.4), respectively, where the lower g values result from coordination through nitrogen rather than oxygen and where the unpaired electron is assigned to the d,, orbital. Case (b) would not occur in a dehydrated copper(I1)-Y zeolite, and case (c) would not be expected to make much of a contribution with copper(I1) ion exchanged zeolites although site I in the hexagonal prism41 could supply an octahedral environment. It is well known that divalent copper does not show an affinity for site 1.2’~~’ Most of the cation sites in Y zeolite have trigonal CaOor D3hsymmetry. It is pertinent to note that Klier et al. have presented calculation^^^ which indicate that the Cu(I1) ions in these locations may lie off of the trigonal axis such that two O(3) (or O(2)) lattice atoms are closer to the cation than the third O(3) (or O(2)) atom. This would correspond to a distorted trigonal symmetry (possibly noncoplanar) with the unpaired electron in the dr2-; or d,, orbital. Although g,, and g, should then be different, it is expected that the difference would be too small to detect using powdered samples. It is of interest to note that gli = g, = 2.252(181) for copper-doped tetrapyridinezinc(I1) pero ~ y d i s u l f a t e where , ~ ~ the distortion is from a square configuration (dx2-; orbital) rather than a tetrahedral one. Partial reduction of highly exchanged Cu(I1)-Y zeolites which had been quickly dehydrated yielded the same EPR parameters as those observed for activated samples of low Cu(I1) content that had been subjected to a prolonged evacuation treatment (hyperfine splittings of about 125 and 160 G, see Figures 2A and 3B). Since this is true when using either H2 or CO as the reducing agent, it appears that the EPR parameters derived from the extensively evacuated samples were not due to Cu(OH), species. Partial reoxidation of the reduced materials at either ambient temperature or at elevated temperatures using O2 or NO regenerated the same spectra, the EPR parameters of which are now attributed to divalent copper ions located in the small cages since these ions are the last ones to undergo reduction, However, the behavior of the lower Cu(1P)-containing Y zeolites was somewhat different. Although the exhibited All values for the latter samples that had been subjected to prolonged evacuation followed by activation, partial reduction, and reoxidation fit the pattern described above, e.g., see Figure 3A, the CuY 5 17 samples that were quickly dehydrated did not. These samples yielded hyperfine splittings of approximately 110 and 175 G as reported in Table IV. Upon reoxidation with NO (Figure 4) or O2 at ambient or elevated temperature, the latter All values were regenerated. This suggests that the location of copper ions in Y zeolites is dependent upon the exchange level (that is, upon the number of sodium ions, which can block the 6-ring windows between the supercage and sodalite units, that remain in the unit cell), as well as the sample treatment. Consideration of the Redox Cycle and Cation Locations. The above discussion demonstrates that the activation technique employed determines the location of the remaining copper(I1) ions in partially reduced Cu-Y zeolites, where all of the zeolites under consideration were exchanged with the divalent cation from aqueous solutions using short equilibration times. Following complete re-
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978 727
duction at high temperatures, reoxidation resulted in the observation that the first reoxidized copper(I1) ions were located in the same type of sites as those occupied by the last Cu(I1) ions to undergo reduction. This was demonstrated by the following events: (a) prolonged evacuation of CuY-10 prior to thermal treatment resulted in the same EPR parameters ’ [gill = 2.37(125),g L 1 = 2.06(20),g1I2= 2.32(160),and gL2= 2.031 after activation, after partial reduction by hydrogen, as well as after reoxidation by oxygen following complete reduction; (b) “fast” evacuation of CuY-10 for 1h prior to thermal treatment resulted in a different but constant set of EPR parameters [gill = 2.38(110),g,’ = 2.06(20), g1I2= 2.30(175),and gL2= 2.031 following the same three treatments as in case (a); (c) “fast” evacuation of CuY-10 prior to thermal treatment resulted in the same EPR parameters as those for case (b) when carbon monoxide rather than hydrogen was used as the reductant and nitric oxide was used as the oxidant instead of oxygen; (d) “fast” evacuation of highly exchanged samples, e.g., CuY-32,60,and 68, resulted in the EPR parameters given in case (a) upon partial reduction with hydrogen and after partial reoxidation by oxygen following complete reduction of Cu(I1) ions; (e) “fast” evacuation of CuY-60 resulted in the same EPR parameters as cases (a) and (d) following partial reduction by carbon monoxide and after partial reoxidation with nitric oxide at ambient temperature following complete reduction of the copper(I1) ions. Thus, these examples show that the zeolites exhibit a memory effect or that some of the copper ions were reduced in place and did not undergo migration even at 773 K during the reduction. The possible mechanisms for the hydrogen reduction of Cu-Y zeolites have been previously d i s c ~ s s e d The .~~~~~~~~ quantity of hydrogen consumed during a mild reduction is approximately stoichiometrically equivalent to the number of copper ions reduced to the univalent and the rate-limiting step has been suggested to be the migration of Cu(I1) ions from the small cages to the supercages where reduction occurs.44 This is expected to be true also when the larger CO molecule is used as the reductant. Support for this is provided by the general observations that the presence of water increases the rate of hydrogen reduction and the presence of ammonia increases the rate of carbon monoxide reduction of divalent copper. However, it would appear that the Cu(1) ions can easily migrate back into the small cages since the ratedetermining step for further reduction and for reoxidation has been proposed to be the migration of the univalent cation from the small cages back into the super cage^.^^ This might again suggest a memory effect of the Y zeolite lattice. Hydrogen reduction of Cu-Y zeolites under more severe conditions results in a hydrogen consumption that can approach the quantity required for complete reduction of Cu(I1) to CU(O).~~ It has been shown for highly exchanged Cu-Y zeolites that at 673 K the reduction to metallic copper is i n ~ o m p l e t e and l ~ ~some ~ ~ of the consumed hydrogen is held in a copper hydride although large (on the order of 30 nm) copper crystallites are found. It has now been demonstrated that the reoxidation of Cu(O), as well as of the copper hydride species, resulted in the regeneration of the EPR spectra obtained after the initial activations. In the cases where a quantity of CuO was
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978
formed upon reoxidation, an additional prolonged or more severe reoxidation converted at least part of the CuO into the desired lattice-held copper(I1) ions. The memory effect might, at first thought, simply depend upon the localized formation of hydroxyl groups or oxygen vacancies created during the reduction process. Although hydroxyl groups and water have been shown by infrared and volumetric techniques to be qualitatively presence after reduction of Cu-Y zeolites,17 a study utilizing diffuse reflectance spectroscopy has failed to detect these moieties following prolonged reduction, where the method is estimated to be able to detect 0.01 water molecule and 0.1 hydroxyl group per copper atom.& In addition, it might be expected that simple oxidation of the Y zeolite by oxygen should destroy any hydroxyls or lattice oxygen vacancies present. Thus, the possible memory effect requires further investigation. Figure 4 and Table V demonstrate that, upon reoxidation of a reduced CuY-10 sample that had been quickly evacuated initially, the first hyperfine splitting value observed was A I = 109 G. This was followed by the appearance of AI[= 172 G and then by AI? = 122 G. This was the same order observed for quickly evacuated activated samples as the copper(I1) content was sequentially increased (Table IV). Upon prolonged evacuation of CuY-10, Ail2= 160 G was observed to be more intense than Ail1= 120 G (Figure 2A), which was the same ordering as those observed for partially reduced highly exchanged Cu-Y zeolites (Figures 3B and 5B). These observations show that a certain site in each case is energetically preferred over other sites. However, upon nearly complete reduction of divalent copper ions in these Y zeolites, the intensities of the two sets of lines become approximately equal, refer to Figure 3A. This might indicate that the copper(I1) ions yielding Ail2 = 160 G are slightly more exposed than are those that produce Ail1 = 120 G. This is in contrast to the expectation when considering the sequential appearance of lines for quickly evacuated samples (Table IV) and for the slowly reoxidized samples (Table V and Figure 4),if the assumption is made that the All 120 G hyperfine splitting is due in each case to Cu(I1) ions in the same lattice site. Therefore, an unambiguous assignment of EPR parameters to copper(I1) ions in specific lattice exchange sites cannot yet be made. Correlation with Other Studies. A structure determination has been completed for dehydrated CuY-57 using powder diffraction data,29and the EPR spectrum of such a sample would consist of a single symmetric line, such as the one shown in Figure SA, narrowed by spin exchange interactions between Cu(I1) ions. A low ion exchanged Cu-Y sample dehydrated according to the procedure used for CuY-57 (heated in oxygen before evacuation) would exhibit gill = 2.37(125),g,l = 2.06(20),g1I2 = 2.32(160), and gL2 = 2.03, e.g., see the first entry in Table I. This is also true of the activation treatment reported for the fully exchanged faujasite, for which the locations of the copper ions have been reported.30 Even though the &/A1 ratios are the same within experimental error for the materials used in the structural studies, the distribution of aluminum atoms might not be the same in the synthetic Y zeolite as in the natural faujasite. However, the reported locations of the Cu(I1) ions in the two structures are in good agreement, e.g., 11.1 Cu2+in site I’29vs. 11.4 and 2.8 Cu2+ ions in I’A and I’B, respe~tively,~~ where I’A corresponds closely to site 1’. This agreement shows that the distributions of aluminum atoms in the natural faujasite and synthetic Y zeolite samples must be very similar. The structure determination of the highly exchanged hydrated Cu(I1)-faujasite, prepared by equilibration in a F;:
R. G. Herman and D. R. Flentge
divalent copper solution for 3 weeks at ambient temperature, indicated the presence of 6.3 Cu(I1) ion/unit cell in the sodalite cage in site 1’, while the remaining metal ions were not locateda30 From consideration of ion exchange data, it has been proposed that in low Cu(I1) exchanged Y zeolite samples prepared by using equilibration times of 2 weeks, the aquocopper(I1) complexes are preferentially held in the sodalite cages.47 In contrast, an equilibration time of 16 h yielded Cu-Y samples in which the supercages contained all of the aquocopper(I1) species.48 Following activation, most of the divalent ions were located in the small This agrees with a recent study of the conductivity and dielectric dispersions of a few zeolites in which relaxation measurements on a dehydrated Cu(I1)-Y zeolite indicated copper migration within the sodalite unit.49 Since the Cu-Y zeolites in the present study were prepared by equilibration in the exchanging solutions for only 4 h, the proposal that the Cu(II)-aquo complexes are in the supercages is in agreement with the sitings previously reported. The copper(I1) ion exchange process in Y zeolites appears to be analogous to the two steps (fast and slow) observed for the exchange of Ca2+into Na-X z e ~ l i t ewhere , ~ ~ ~the ~ slow step is the migration of Ca2+into the small cages.
Conclusions When the ion exchange of Na-Y zeolites with low concentrations of copper(I1) is carried out at ambient temperature with short equilibration times, e.g., 4 h, the exchanged hydrated copper(I1) ions are located in the supercages. The free rotation of these complexes is hindered, probably by orientation through hydrogen bonding between the coordinated water and the negatively charged zeolite lattice. It appears that rapid dehydration tends to leave the divalent cations in the supercages, where the cations exhibit distinctive EPR parameters, but slow dehydration by prolonged evacuation allows the Cu(I1) ions to migrate into the small cages. Following activation, cations in the latter positions exhibit a different distinctive set of EPR parameters and are the last divalent ions to undergo high temperature reduction. As the Cu(I1) content of the zeolite increases and the Na+ content decreases, rapid dehydration tends to yield copper(I1) ions located in both supercage and small cage sites. The EPR parameters obtained upon partial reduction and reoxidation are the same as those exhibited by the particular sample following one of the dehydration procedures prior to reduction. Thus, the number of Na+ ions remaining in the zeolite, the time of equilibration used for the Cu(I1) ion exchange, and the dehydration procedure can influence the location of copper(I1) ions in Y zeolites, and the diverse hyperfine splitting values exhibited in Table I are now understandable.
Acknowledgment. We sincerely thank Dr. Jack H. Lunsford for the use of his facilities, for constructive discussions, and for partial support of this research through National Science Foundation Grant NO. CHE-74-08660. We appreciate the helpful and instructive discussions with Dr. Kamil Klier of Lehigh University. Portions of this paper were presented at the 7th Northeast Regional Meeting of the American Chemical Society, Albany, N.Y., August 1976, Abstract No. 252 and at the 9th Central Regional Meeting of the American Chemical Society, Charleston, W.Va., October 1977, Abstract No. INOR-35. References and Notes (1) Present addresses: (a) Center for Surface and Coatings Research, Sinclair Laboratory No. 7, Lehigh University, Bethlehem, Pa. 18015;
ESR Study of Metal-Ammonia Solutions (b) Tennessee Temple Schools, 1815 Union Avenue, Chattanooga, Tenn. 37404. (2) C. Naccache and Y. Ben Taarit, J . Chem. Soc., Faraday Trans. 7, 69, 1475 (1973). (3) T. J. Barry and L. A. Lay, J. fhys. Chem. Solids, 29, 1395 (1968). (4) N. N. Tikhomirova, I.V. Nikolaeva, V. V. Demkin, E. N. Rosolovskaya, and K. V. Topchieva, J . Catal., 29, 105,500 (1973). (5) J. W. Jermyn, T. J. Johnson, E. F. Vansant, and J. H. Lunsford, J . fhys. Chem., 77, 2964 (1973). (6) E. G. Derouane, M. Mestdagh, and L. Vielvoye, J . Catal.. 33, 169
(1974). (7) E. F. Vansant and J. H. Lunsford, Adv. Chem. Ser., No. 121, 441 (1973). (8) K. A. Windhorst and J. H. Lunsford, J. Am. Chem. Soc., 97, 1407 (1975). (9) R. F. Howe and J. H. Lunsford, J. Am. Chem. Soc., 97, 5156 (1975). (10) P. H. Kasai and R. J. Bishop, Jr., J. Phys. Chem., 77,2308 (1973). (11) H. B. Slot and J. L. Verbeek, J . Catal., 12, 216 (1969). (12) J. T. Richardson, J . Catal., 9, 178 (1967). (13) U. Kruerke and P. Jung, Z . Phys. Chem. (Frankfurt am Main), 58, 53 (1968). (14) D. d. Flentge, J. H. Lunsford, P. A. Jacobs, and J. B. Uytterhoeven, J. fhys. Chem., 79, 354 (1975). (15) J. Turkevich, Y. Ono, and J. Soria, J. Catal., 25, 44 (1972). (16) C. Naccache and Y. Ben Taarit, Chem. Phys. Lett.. 11, 1 1 (1971). (17) R. G. Herman, J. H. Lunsford, H. Beyer, P. A. Jacobs, and J. B. Uytterhoeven, J. Phys. Chem., 79,2388 (1975). (18) E. F. Vansant and J. H. Lunsford, J . Phys. Chem., 76, 2860 (1972). (19) I.E. Maxwell and E. Drent, J. Catal., 41, 412 (1976). (20) A. Nlcula, D. Stamires, and J. Turkevich, J. Chem. Phys., 42, 3684 (1965). (21) N. G.Makslmov, U. F. Anufrlenko, K. G. Ione, and N. A. Shestakova, Zh. Strukt. Khim., 13, 1020 (1972);Engl. Trans., p 953. (22) I.D. Mikhelkin, V. A. Shvets, and V. B. Kazanskii, Kinet. Katal., 11, 747 (1970);Engl. Trans., p 609. 1231 R. Kellermanand K. Klier in “Surface and Defect Prooerties of SolMs”. Vol. 4,M. W. Roberts and J. M. Thomas, Ed., Biliing & Sons Ltd., London, 1975,pp 1-33. (24) R. Kellerman, P. J. Hutta, and K. Klier, J. Am. Chem. Soc., 96,5946 (1974). I
The Journal of Physical Chemistry, Vol. 82, No. 6, 1978 729
(25) R. Y. Yanagida, T. B. Vance, Jr., and K. Seff, Inorg. Chem., 13, 723 (1974). (26) K. Klier, Adv. Chem. Ser., Ne. 101, 480 (1971). (27) P. E. Riley and K. Seff, Inorg. Chem., 13, 1355 (1974). (28) K. Klier and M. Rllek, J. Phys. Chem. Solids, 29, 951 (1968). (29) P. Gallezot, Y. Ben Taarit, and B. Imelik, J. Catal., 26, 295 (1972). (30) I. E. Maxwell and J. J. de Boer, J . fhys. Chem., 79, 1874 (1975). (31) C. C. Chao and J. H. Lunstord, J. fhys. Chem., 76, 1546 (1972). (32) W. 8. Lewis, M. Alei, Jr., and L. 0. Morgan, J . Chem. Phys., 44, 2409 (1966). (33) C. HeRner-Wirauin and R. Cohen, J . Phys. Chem., 71, 2556 (1967). (34) K. Umezarva and T. Yamabe, Bull. Chem. Soc. Jpn., 45, 56 (1972). (35) A. Hudson, Mol. Phys., 10, 575 (1966). (36) B. R. Mc Garvey in “Transition Metal Chemistry”, Vol. 3,R. L. Carlin, Ed., Marcel Dekker, New York, N.Y., 1966,pp 89-201. (37)G. Vierke, J . Chem. SOC.,Faraday Trans. 7 , 69, 1523 (1973). (38) B. J. Hathaway and D. E. Billing, Coord. Chem. Rev., 5, 143 (1970). (39)G.F. Kokoszka, C. W. Reimann, and H. C. Allen, Jr., J. fhys. Chem., 71, 121 (1967). (40) S.N. Choi, R. D. Bereman, and J. R. Wasson, J. Inorg. Nucl. Chem., 37, 2087 (1975). (41) For a discussion of the positions of and nomenclature used for lattice sites see J. V. Smlth, Adv. Chem. Ser., No. 101, 171 (1971). (42) K. Klier, P. J. Hutta, and R. Kellerman, ACS Symp. Ser., 40, 108 (1977). (43) H. G. Hecht and J. P. Frazier, 111, J. Chem. fhys., 44, 1718 (1966). (44) P. A. Jacobs, M. Tielen, J.-P. Linart, J. B. Uytterhoeven, and H. Beyer, J . Chem. Soc., Faraday Trans. 7, 72, 2793 (1976). (45) J. Texter, D. H. Strome, R. G. Herman, and K. Klier, J. fhys. Chem., 81, 333 (1977). (46) L. Riekert, Ber. Bunsenges. fhys. Chem., 73, 331 (1969). (47) A. Maes and A. Cremers, J. Chem. Soc., Faraday Trans. 1 , 71, 265 (1975). (48) P. P. Lai and L. V. C. Rees, J. Chem. Soc., Faraday Trans. 7, 72, 1809 (1976). (49) R. A. Schoonheydt, W. De Wilde, and F. Velghe, J . fhys. Chem., 80. 511 (1976). (50) R. M. Bairer, J.’A. Davies, and L. V. C. Rees, J. Inorg. Nucl. Chem., 31, 2599 (1969). (51) H. S. Sherry, Adv. Chem. Ser., No. 101, 350 (1971).
Metal-Ammonia Solutions. 10. Electron Spin Resonance. A Blue Solid Containing a Crown Ether Complexing Agent R. L. Harris and J. J. Lagowski” Welch Chemical Laboratory, The University of Texas, Austin, Texas 78712 (Received October 27, 7977)
The results of ESR measurements on liquid and frozen solutions of potassium and 18-crown-6 in ammonia are reported. The results for the liquid state are similar to those previously reported for solutions without 18-crown-6. Three features are observed for frozen solutions which can be explained in terms of two different types of potassium metal species and an ion pair consisting of a “solvated” electron and the potassium cation complexed by the crown moiety. The implications of these results for liquid solution ESR spectra of metal-ammonia solutions are discussed.
Introduction During the course of extensive studies of metalammonia solutions’ a number of unusual properties have been discovered. Among the more interesting magnetic properties of these solutions is the narrowness of the electron resonance absorption line. In the most widely accepted theory, the ESR results are explained in terms of motional narrowing of the hyperfine interaction with nitrogen nuclei.2 A better understanding of the solvated electron in liquid ammonia could be obtained if a detailed analysis were available on a similar species in the solid state. Many attempts3 have been made to isolate the ammoniated
electron in the solid state. Various paramagnetic species can be isolated from ammonia and hexamethylphosphorous triamide as trapped paramagnetic centers, but the large number of such species that have been isolated bear little resemblance to those found in solution. Dye and co-workers4have been successful in isolating the sodium anion, a species long presumed to exist in metal-amine solutions, by the judicious use of crown ether complexing agents in ethylamine solutions. Amorphous gold-colored and blue-colored solids have been obtained from a variety of solvents.6 In experiments preliminary to the work reported here we were able to obtain blue solids from liquid ammonia
0022-365417812082-0729$01.00/0. 0 1978 American Chemical Society